# MSEG 803 Equilibria in Material Systems 12: Solution Theory

## Presentation on theme: "MSEG 803 Equilibria in Material Systems 12: Solution Theory"— Presentation transcript:

MSEG 803 Equilibria in Material Systems 12: Solution Theory
Prof. Juejun (JJ) Hu

Gibbs theorem 1 Solid 1 consisting of N1 atoms on N1 lattice sites Solid 2 consisting of N2 atoms on N2 lattice sites Solid solution with the same lattice structure and completely random distribution of atoms Inter-atomic force are the same for all three types of atomic pairs: 1-1, 2-2, and 1-2 2 1+2

Gibbs theorem 1 2 1+2 Ideal (random) solid solution Entropy of mixing
The entropy of mixing is also consistent with the informational theory definition of entropy 1+2

Gibbs theorem for ideal gas
Entropy of mixing ideal gases (at the same T and P): Derivation: # of spatial “sites” m >> # of molecules n for ideal gas (classical limit of quantum statistics) T, P, n1 T, P, n2 Same T and P :

Ideal solid solutions Inter-atomic force is the same for all types of bonds Random mixing is always preferred!

Regular binary solution theory
Assumptions: Random distribution of atoms Bond energy between 1-2 is different from those of 1-1 and 2-2 negative enthalpy of mixing: 1-2 type of hetero-polar bond energetically favorable positive enthalpy of mixing: 1-1 and 2-2 types of homopolar bonds preferred 1 2 Site i Site j

Negative enthalpy of mixing

Positive enthalpy of mixing (high T)

Positive enthalpy of mixing (intermediate T)

Positive enthalpy of mixing (low T)

The intercept rule The chemical potentials of components 1 and 2 are given by the intercept of the tangent line of the Gibbs free energy curve G m1 G(x1, x2) m2 x1 Pure 2 x1, x2 Pure 1

Phase composition determination
The composition of phases are determined by the common tangent lines on the Gibbs free energy curve Minimization of G The curve is generally asymmetric for non-ideal solution solutions DGmix at T = T0 a b m2 m1 x1,a x1,b

Phase diagram Gibbs free energy Miscibility gap Miscible region
Convex G curve: miscible solution Miscibility gap: the bond energy gain of homopolar bond formation dominates over the entropy of mixing Gibbs free energy Concave G curve: phase separation

Miscibility gap in Au-Ni alloy phase diagram

Short range order (SRO)
Regular solution theory: random distribution of atoms Probability of forming 1-2 is the same as that of forming 1-1 and 2-2 bonds Large negative enthalpy of mixing Bond energy of 1-2 bonds is much larger than average bond energy of 1-1 and 2-2 bonds Heteropolar bonds strongly preferred over homopolar bonds SRO maximizes the number of 1-2 hetero-polar bonds Binary phase with SRO at low T (DHmix dominates the contribution to DGmix) 1 2 Site i Site j

Short range order (SRO)
B2 ordering in BCC structures (atom 1 and 2 molar ratio 1:1) Ordering in molar ratio 1:1 FCC structures is impeded by tetrahedral units

Short range order (SRO)
Miscibility gap due to positive DHmix SRO phase x1 x1 Experimental validation of SRO phase formation vs. miscibility gap due to positive DHmix Structural characterization Calorimetry measurement

Completely miscible solid/liquid solution
G (at T = T1) T T1 l s l s x1 x1 Pure 2 Pure 1 Pure 2 Pure 1 Liquid and solid phases each has its own G curve Liquid phase has molar lower Gibbs free energy at high T

Completely miscible solid/liquid solution
G (at T = T2) T s l m1 l T2 s m2 x1 x1 Pure 2 x1,l x1,s Pure 1 Pure 2 x1,l x1,s Pure 1 Liquid and solid phases each has its own G curve Equilibrium phase composition is determined by the common tangent line

Completely miscible solid/liquid solution
G (at T = T3) T l l s s x1 T3 x1 Pure 2 Pure 1 Pure 2 Pure 1 The term is larger (less negative) for solids; thus at low T solid becomes the stable phase

Eutectic phase diagram
G (at T = T1) T T1 a b l l a b x1 x1 Pure 2 Pure 1 Convex liquid phase Gibbs free energy curve lies everywhere below the G curves of a and b phases: homogeneous liquid phase l

Eutectic phase diagram
G (at T = T2) T a b l l T2 a b x1 x1 Pure 2 Pure 1 Compositions of l, a and b phases are determined by the common tangents

Eutectic phase diagram
G (at T = T3) T a b l l T3 a b x1 x1 Pure 2 Pure 1 Compositions of l, a and b phases are determined by the common tangent Three phases share a common tangent at eutectic T

Eutectic phase diagram
G (at T = T4) T a l l b a b T4 x1 x1 Pure 2 Pure 1 Compositions of a and b phases are determined by the common tangent